| ||Format||Pages||Price|| |
|4||$46.00||  ADD TO CART|
|Hardcopy (shipping and handling)||4||$46.00||  ADD TO CART|
Significance and Use
4.1 The amount of ferrite present in an austenitic stainless steel has been shown to influence the strength, toughness, and corrosion resistance of this type of cast alloy. The amount of ferrite present tends to correlate well with the magnetic permeability of the steel. The methods described in this standard cover calibration practice for estimating ferrite by the magnetic permeability of the steel. The practice is inexpensive to use over large areas of the cast part and is nondestructive.
4.2 This practice has been used for research, alloy development, quality control, and manufacturing control.
4.2.1 Many instruments are available having different designs and different principles of operation. When the probe is placed on the material being investigated, a closed magnetic circuit is formed allowing measurement of the magnetic permeability. When calibrated with standards having known ferrite content, this permeability indicates the ferrite content of the material being analyzed. The estimated ferrite content is read from a calibrated dial or from a digital readout dial. Follow the manufacturer's instructions for proper calibration of the instrument.
4.3 Since this practice measures magnetic attraction and not ferrite directly, it is subject to all of the variables that affect magnetic permeability, such as the shape, size, orientation, and composition of the ferrite phase. These in turn are affected by thermal history. Ferrite measurements by magnetic methods have also been found to be affected by the surface finish of the material being analyzed.
4.4 Magnetic methods should not be used for arbitration of conflicts on ferrite content except when agreed upon between manufacturer and purchaser.
1.1 This practice covers the procedure for calibration of instruments to be used for estimating the ferrite content of the microstructure of cast stainless steels by magnetic response or measurement of permeability. This procedure covers both primary and secondary instruments.
1.1.1 A primary instrument is one that has been calibrated using National Institute of Standards and Technology-Standard Reference Material (NIST-SRM) thickness coating standards. It is a laboratory tool to be used with test specimens. Some primary instruments may be used to directly measure the ferrite content of castings.
1.1.2 A secondary instrument is one that has been calibrated by the use of secondary standards that have been measured by a calibrated primary instrument. Secondary instruments are to be used to directly measure the ferrite content of castings.
1.2 The values stated in either SI units or inch-pound units are to be regarded separately as standard. The values stated in each system may not be exact equivalents; therefore, each system shall be used independently of the other. Combining values from the two systems may result in nonconformance with the standard.
1.2.1 Within the text, the SI units are shown in brackets.
1.3 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use.
1.4 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
A941 Terminology Relating to Steel, Stainless Steel, Related Alloys, and Ferroalloys
B499 Test Method for Measurement of Coating Thicknesses by the Magnetic Method: Nonmagnetic Coatings on Magnetic Basis Metals
E562 Test Method for Determining Volume Fraction by Systematic Manual Point Count
ICS Number Code 77.140.80 (Iron and steel castings)
UNSPSC Code 31100000(Castings and casting assemblies)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM A799 / A799M-10(2020), Standard Practice for Steel Castings, Stainless, Instrument Calibration, for Estimating Ferrite Content, ASTM International, West Conshohocken, PA, 2020, www.astm.orgBack to Top